Ó Operative Dentistry, 2012, 37-2, 000-000 Selective Enamel Etching: Effect on Marginal Adaptation of Self-Etch LED-Cured Bond Systems in Aged Class I Composite Restorations EJ Souza-Junior LT Prieto CTP Araujo ´ LAMS Paulillo Clinical Relevance Selective enamel etching was shown to be an effective approach to reduce gap formation in Class I composite restorations for one-step self-etch adhesives.SUMMARY seconds with 37% phosphoric acid; the otherThe aim of this study was to evaluate the half were not etched. For the photoactivationinfluence of previous enamel etch and light of the adhesives and composite, three light-emitting diode (LED) curing on gap formation curing units (LCUs) were used: one polywaveof self-etch adhesive systems in Class I com- (Ultra-Lume LED 5, UL) and two single-peakposite restorations after thermomechanical (FlashLite 1401, FL and Radii-cal, RD) LEDs.aging (TMA). Thus, on 192 human molars, a After this, epoxy resin replicas of the occlusalbox-shaped Class I cavity was prepared main- surface were made, and the specimens weretaining enamel margins. Self-etch adhesives submitted to TMA. New replicas were made(Clearfil SE and Clearfil S3) were used to from the aged specimens for marginal adapta-restore the preparation with a microhybrid tion analysis by scanning electron microscopy.composite. Before application of the adhesives, Data were submitted to Kruskal-Wallis andhalf of the teeth were enamel etched for 15 Wilcoxon tests (a=0.05). Before TMA, when enamel was etched before the application of*Corresponding author: Piracicaba Dental School, State S3, no gap formation was observed; however, University of Campinas – UNICAMP there were gaps at the interface for the otherDepartment of Restorative Dentistry, Av. Limeira, 901, tested conditions, with a statistical difference ˜ ˜Areiao, PO Box: 52, Piracicaba, Sao Paulo 13414-903 Brazil;email@example.com (p0.05). After TMA, the selective enamel etch- ing previous to the S3 application, regardlessDOI: 10.2341/11-184L of the LCU, promoted higher marginal adapta-
2 Operative Dentistrytion compared to the other tested groups ensure a good bond performance and marginal(p0.05). Prior to TMA, higher marginal integ- integrity. An efficient light-curing unit (LCU) shouldrity was observed, in comparison with speci- guarantee a satisfactory adhesive and compositemens after TMA (p0.05). With regard to degree of conversion, which may improve its physicalClearfil SE and Clearfil Tri-S cured with FL, and mechanical properties, yielding a good marginalno differences of gap formation were found seal.18-22 Quartz-tungsten-halogen (QTH) lampsbetween before and after aging (5.3 6 3.8 and have been largely used in restorative procedures;7.4 6 7.5, respectively), especially when the however, they present some drawbacks like bulb,Clearfil Tri-S was used in the conventional filter, and reflector degradation over time and aprotocol. When cured with RD or UL and not lifetime of approximately 40 to 100 hours.18-20 In thisetched, Clearfil Tri-S presented the higher gap sense, light emitting diodes (LEDs) have been shownformation. In conclusion, additional enamel to overcome these problems, promoting an adequateetching promoted better marginal integrity for cure of resin composites and dental adhesivesClearfil Tri-S, showing it to be an efficient through emission of unfiltered blue light.18-20 Thesetechnique for Class I composite restorations. LCUs generate a narrow spectral range that targetsThe two-step self-etch adhesive was not influ- the absorption wavelength of camphorquinone,enced by selective enamel etching or by the yielding low amounts of wasted energy and mini-LED-curing unit. mum heat generation, with a longer lifetime and less decrease of light intensity.18-20 Thus, the curing INTRODUCTION potential of current LED curing units has beenComposite restorations have been widely used in shown to be similar to that presented by conven-clinical practice, due to esthetic and some biome- tional QTH light units.23-25chanical properties similar to dental hard tissues.1 It is known that some resinous materials, likeFor the bonding procedure of these adhesive resto- resin cements, and some adhesive systems are notrations, self-etching bond systems were introduced well cured with conventional single-peak LEDs dueto decrease the number of bonding technical steps,since the presence of acidic monomers in their to alternative photoinitiator content.26 Because ofcomposition yields simultaneous etching and prim- this, LEDs with additional wavelengths (polywaveing of the dental hard tissues.2,3 A partial removal of third generation LEDs) were developed, emittingthe smear layer is promoted and, consequently, the light wavelengths within a spectral region thatformation of smear plugs left undisturbed, decreas- targets the absorption peak of camphorquinone anding tooth postoperative sensitivity and leaving the within the UV-VIS region (400–415 nm).23-25 Thisadhesive protocol less time-consuming.3-6 polywave behavior is expected to yield an adequate cure of adhesives and composites that contain Self-etching adhesives are known to exhibit a good alternative photoinitiator systems, such as phenylbonding performance to dentin and a poor bonding propanedione, bis-alkyl phosphinic oxide, and trime-behavior to enamel.3,4 In order to remove the smear thylbenzoyl-diphenyl-phosphine oxide.25 Since man-layer created by instrumentation, demineralize the ufacturers do not state all photoinitiator content, isenamel substrate, and increase bond quality anddurability, a selective enamel phosphoric acid etch- it important to choose an adequate LCU that woulding before the application of a self-etch adhesive has polymerize all resinous materials,25-27 enhancing thebeen proposed.7-11 Some studies demonstrated that marginal seal and improving the composite restora-this additional enamel etching decreases gap forma- tions’ durability.tion when self-etch adhesives are used.5,6,12-16 Thus, this study aimed to investigate the influenceHowever, this additive step for direct composite of prior enamel etching and LED curing lights onrestoration procedures was only evaluated in Class gap formation of self-etch bond systems in Class III, III, and V restorations.5,6,13-16 Since the Class I composite restorations. The first tested hypothesispreparation exhibits a high Configuration factor was that selective enamel etching would improve thewith enamel surrounding the superficial margins, marginal adaptation of the adhesive systems init is considered the best model for understanding the Class I composite restorations. The second hypoth-real effects of enamel etching and the stress esis was that the third generation polywave LEDdevelopment on the tooth/adhesive interface.14,17 would present lower gap formation for the tested An adequate bond system cure is another impor- bond systems. Moreover, the third hypothesis wastant factor to consider in restoring Class I cavities to that the thermomechanical fatigue would increase
Souza-Junior Others: Effect of Enamel Etching on Marginal Adaptation of Composite Restorations 3 Table 1: Composition, Application Mode, and Manufacturers’ Information for the Adhesive Systems Tested Adhesive Systems Composition Application Mode Clearfil SE Bond (Kuraray Medical Inc, Primer (batch 00896A): water, MDP, HEMA, Apply primer for 20 seconds. Mild air Tokyo, Japan) camphorquinone, hydrophilic dimethacrylate. stream. Apply bond. Gentle air stream. Light cure at an energy density of 11 J. Adhesive (batch 01320A): MDP, bis-GMA, HEMA, camphorquinone, hydrophobic dimethacrylate, N,N-diethanol p-toluidine bond, colloidal silica. Clearfil Tri-S Bond (Kuraray Medical Adhesive (batch 00116A): MDP, bis-GMA, HEMA Apply the bond system for 20 seconds. Inc, Tokyo, Japan) hydrophobic dimethacrylate, dl-camphorquinone, Gentle air stream for 10 seconds. Light silanated colloidal silica, ethyl alcohol, and water. cure at an energy density of 11 J. Charisma (Heraeus Kulzer, Hanau, Composite (batch 010080): Bis-GMA, TEGDMA, Light cure at an energy density of 22 J. Germany) barium aluminum boro silicate glass and pyrogenic silicon dioxide, photoinitiators (64% filler),interfacial debonding, promoting higher gaps at the Culver City, CA, USA), Radii-cal (RD) (SDI Limited,superficial margins. Victoria, Australia), and Ultra-Lume LED 5 (UL) (Ultradent, South Jordan, UT, USA). Prior to the MATERIALS AND METHODS restorative procedure, the output power (mW) ofOne hundred ninety-two healthy human third each LCU was measured with a calibrated powermolars were selected. The teeth were collected after meter (Ophir Optronics, Har, Hotzvim, Jerusalem,obtaining the patient’s informed consent under a Israel). Then, irradiance (mW/cm2) was determinedprotocol approved by the State University of Campi- by dividing the output power by the tip end area.nas ethical review board (057/2009). The teeth were Spectral distributions were measured with a cali-cleaned, embedded in polystyrene resin, and their brated spectrometer (USB2000, Ocean Optics, Dun-occlusal surfaces were wet polished with 320-grit SiC edin, FL, USA). Beam distribution and irradiancepaper under running water (Politriz, AROTEC, Sao ˜ data were integrated using the Origin 6.0 softwarePaulo, Brazil) to expose a flat enamel surface area (OriginLab, Northampton, MA, USA). The spectralwithout exposing dentin. Then, typical Class I range distribution of each LCU is shown on Figure 1,cavities were prepared using no. 56L carbide burs and the characteristics of the LCUs are presented in(KG Sorensen, Barueri, Brazil) at high-speed, underair/water cooling. After five-cavity preparations, thebur was replaced. Preparations had a standard size,with cavity dimensions of 5 mm mesial-distally, 5mm buccal-lingually, and a 3 mm depth, maintain-ing all cavity margins on enamel substrate. Two self-etch adhesive systems were used for the bondingprotocols: Clearfil Tri-S Bond (one-step self-etch, pH= 2.7, Kuraray Medical Inc, Okayama, Japan) andClearfil SE Bond (two-step self-etch, pH = 2,Kuraray Medical Inc). The composition, applicationmode, and batch number of the adhesive systems arepresented in Table 1. After cavity preparation, teethwere assigned to 12 groups (n=16) according to thethree studied factors: selective enamel etching, bondsystem, and curing light (two conditioning protocols3 two adhesives 3 three LEDs). For the photoactivation procedure three LEDs Figure 1. The spectral range distribution of each LCU used in thiswere tested: FlashLite 1401 (FL) (Discus Dental, study.
4 Operative Dentistry Table 2: Characteristics of the Light-Curing Units (LCUs) Used in This Study LCU Manufacturer Type Tip Diameter, Irradiance, Composite Radiant Adhesive Radiant mm mW/cm2 Exposure, J/cm2 Exposure, J/cm2FlashLite 1401 Discus Dental, Culver City, Single-peak 7 1077 22 11 CA, USARadii-cal SDI Limited, Victoria, Single-peak 7 731 22 11 AustraliaUltra-Lume LED 5 Ultradent Products Inc, Polywave 11 3 7 800 22 11 South Jordan, UT, USATable 2. Also, energy density was standardized to scanning electron microscope (JEOL, JSM-5600LV,approximately 11 J for curing the bonding system Tokyo, Japan) at 2003 magnification. SEM analysisand 22 J for each composite increment photoactiva- of the composite/enamel marginal adaptation wastion. For RD, due to the fact that it mandatorily performed by one operator having experience withoperates in ramp mode for 5 seconds, these initial quantitative margin examination and who wasseconds were discarded, and only a continuous light blinded to the restorative procedures. The marginalwas delivered to keep the irradiance standardized. integrity between resin composite and enamel wasConsequently, an equal energy density was obtained expressed as a percentage of the entire superficialfor each of the LCUs. margin length. All groups were restored with B1-shade Charismamicrohybrid composite (Heraeus Kulzer, Hanau, Enamel Etching PatternsGermany), using an incremental oblique techniquewith six increments of approximately 2 mm thick. Eighteen half-teeth (n=3 for the two self-etchThe first layer was applied horizontally and light adhesives with and without prior enamel etch andcured, followed by two oblique layers. Next, another negative and positive controls) were ground andthree layers were placed in the same way as randomly assigned into 12 groups. For the positivedescribed before, until the cavity was completely control, a 37% phosphoric acid treatment wasfilled. Then, finishing and polishing procedures were realized and for the negative control, the enamelperformed with medium-, fine-, and extra fine-grit surface did not receive any treatment. The experi-aluminum oxide disks (SoftLex, 3M/ESPE, St Paul, mental groups were treated with the two tested bondMN, USA), respectively. After polishing, impressions systems using manufacturer’s instructions with orwith a low viscosity vinyl polysiloxane material without prior enamel etching. The treated surfaces(Express XT, 3M ESPE) of the teeth were taken were thoroughly rinsed with alternate baths ofand a first set of epoxy resin replicas (Epoxicure acetone (20 seconds) and ethanol (20 seconds) in anResin, Buehler, Lake Bluff, IL, USA) was made for attempt to remove the self-etch primers and thescanning electron microscopy (SEM) evaluation. In monomer components. All specimens were dehydrat-sequence, specimens were submitted to 200,000 ed in ascending grades of ethanol (25%, 50%, 75%,mechanical loading of 40N (2 Hz) and 500 thermal and 90%) for 10 minutes each and immersion incycles (ranging from 58C to 558C with a dwell time of 100% ethanol for 30 minutes. After dry storage at60 seconds in each bath with an interval of 5 378C for 24 hours, specimens were sputter coatedseconds) in a thermomechanical device ER-11000 with gold and analyzed by SEM. ˜(ERIOS, Sao Paulo, Brazil) to simulate aging of thecomposite restorations in oral environment condi- Statistical Analysistions. For the statistical analysis, as the data did not New impressions of the teeth were made and exhibit normal data distribution (Kolmogorov-Smir-another set of replicas was made for each restora- nov test), nonparametric tests were used (Kruskal-tion. All replicas were mounted on aluminum stubs, Wallis for groups’ comparison and Wilcoxonsputter coated with gold, and evaluated with a matched-pairs signed-rank tests for pairwise com-
Souza-Junior Others: Effect of Enamel Etching on Marginal Adaptation of Composite Restorations 5 Table 3: Results of the Gap Formation Analysis (% and integrity and marginal gaps of Class I composite SD) of Enamel Margins Before and After restorations that were observed in this study. Thermomechanical Aging) Prior to thermomechanical loading, higher mar- ginal integrity was observed in comparison with Tested Conditions Before Aging, After Aging, after aging (Wilcoxon test; p0.05). When the % (SD) % (SD) bonding systems were cured with FL and only when Clearfil Tri-S was used in the conventional way wereFlashLite/no etch/Clearfil SE 2.6 (4.7)B 5.6 (4.5)AB* there no differences between before and after aging (5.3 6 3.8 and 7.4 6 7.5, respectively). When curedFlashLite/etch/Clearfil SE 0.6 (1.3)B 3.0 (2.8)AB* with RD or UL and not etched, Clearfil Tri-S presented the higher gap formation.FlashLite/no etch/Clearfil Tri-S 5.3 (3.8)B 7.4 (7.5)AB Enamel Etching PatternsFlashLite/etch/ Clearfil Tri-S 0A 2.4 (4.9)A* The SEM enamel etching patterns are shown in Figures 3 (A,B), 4 (A,B), and 5 (A,B,C).Radii-cal/no etch/Clearfil SE 3.2 (3.9)B 13.1 (14.7)AB* DISCUSSIONRadii-cal/etch/Clearfil SE 3.6 (8.2)B 6.2 (8.6)AB An important factor to promote clinical success ofRadii-cal/no etch/ Clearfil Tri-S 3.0 (3.1)B 12.4 (10.7)B* Class I resin composite restorations is a satisfactory enamel marginal adaptation. The presence of gaps isRadii-cal/etch/ Clearfil Tri-S 0A 2.9 (5.7)A considered as the first sign of restoration failure, clinically evidenced by marginal staining.28 Also,Ultra-Lume/no etch/Clearfil SE 3.5 (4.0)B 3.9 (4.4)AB when detectable marginal disruption is present, these interface defects could lead to interfacialUltra-Lume/etch/Clearfil SE 3.7 (3.7)B 4.8 (4.9)AB leakage.28,29 In the oral environment, many pulpal sensitivities and responses are related to whenUltra-Lume/no etch/ Clearfil Tri-S 3.1 (4.3)B 8.6 (7.5)B* bacterial leakage occurs along the tooth/composite bonding interface.Ultra-Lume/etch/ Clearfil Tri-S 0A 0.9 (2.61)A In the present work, the first hypothesis was Same letters within column indicate no statistically significant difference partially validated, since only the gap formation for (p0.05, Kruskal-Wallis and Dunn comparison). Asterisks stand for p0.05; the one bottle all-in-one self-etch adhesive Clearfil Wilcoxon matched-pairs and signed-rank tests. Tri-S was affected by the selective enamel etching procedure, regardless of the LCU. This may be explained by some characteristics of this mild one-parisons before and after thermomechanical aging) step adhesive, like its pH and etching potential.3,4 Aswith a pre-set alpha of 0.05. shown by SEM evaluation of the enamel etching patterns , Clearfil Tri-S alone promotes a smooth RESULTS enamel demineralization, not increasing the surface free energy and bond penetration. Its pH of approx-Marginal Adaptation Analysis imately 2.6 did not promote an adequate demineral-The results of the marginal adaptation analysis are ization of the enamel surface and resulted in poorshown in Table 3. No gap formation was observed bond strength. This weak bond interface is easilybefore thermomechanical loading when enamel was affected by composite shrinkage stress during theetched before the application of Clearfil Tri-S; photocuring procedure.7,8,28 In this sense, the selec-however, there were gaps at the interface of the tive enamel etch procedure could have promoted aClearfil SE Bond regardless of the energy source, deeper dissolution of prism cores and boundaries in awith statistical difference (Kruskal-Wallis test; type III etching pattern, increasing the surface freep0.05). After aging, selective etching prior to the energy of this substrate and consequently, increas-Clearfil Tri-S application, when RD or UL were used, ing the percentage of gap-free margins.promoted higher marginal adaptation compared to For Clearfil SE Bond, the previous acid etching didthe other tested groups (Kruskal-Wallis test; not affect the gap formation of the compositep0.05). Figure 2 shows examples of marginal restorations. This may have occurred because of
6 Operative DentistryFigure 2. (A): The white arrows point to interfacial gap formed between resin composite and enamel. (B): The white arrows indicate a perfectmarginal seal between enamel and composite. (C): Note the composite/resin interface presenting some interfacial gaps. The white arrows point to thecorrect location of the marginal gaps. (D): A high magnification showing the interfacial gaps between composite and dental enamel.the lower pH of the adhesive system, approximately based resin exhibited a similar behavior as the single-2.0, which could have promoted higher enamel peak second generation LED. This was demonstrateddemineralization compared to Clearfil Tri-S alone, by the fact that both adhesive systems and theregardless of the curing light. Also, the studied two- microhybrid composite with camphorquinone did notstep bond system contains a separate hydrophobic have interfacial integrity affected. Also, they mayresin that is applied after the acidic primer. This have presented a similar degree of cure and conse-hydrophobic resin coat can improve bond durability, quently, less marginal shrinkage stress, preservingespecially due to the structural polymer network the superficial marginal adaptation between compos-that is not hydrophilic and can maintain optimal ite and enamel.bonding behavior after fatigue stress.8,30,31 Another fact to discuss is the morphology of the The second hypothesis of this study was rejected Ultra-Lume LED 5 tip, in which there is a centralbecause the polywave third-generation LED did not LED that emits visible light at the peak spectra ofimprove the marginal adaptation of the resin com- camphorquinone and four accessory LEDs in theposite restorations. The photoinitiator content of the corner of the tip that emit UV-VIS wavelengths. In acomposite and adhesive resin formulations seems to Class I preparation, with 25 mm2, as the conditionbe camphorquinone, as informed by manufacturers. presented in this work, light emitted by theTherefore, the polywave LED for camphorquinone- accessory LEDs would not reach the adhesive resin
Souza-Junior Others: Effect of Enamel Etching on Marginal Adaptation of Composite Restorations 7Figure 3. (A): SEM photomicrograph showing the dental enamel without any acid treatment. (B): Phosphoric acid (37%) etched enamel, showing atype II etching pattern, with the dissolution of the prism cores.since the tip dimensions are higher than the area of ly validating the third hypothesis. When specimensthe tooth preparation.24 Consequently, only the were restored using Clearfil Tri-S without selectivecentral LED with the absorption peak of camphor- enamel etching, the thermomechanical aging pro-quinone may have irradiated the adhesive resin, moted less marginal integrity, except when FL waspromoting similar gap formation as FlashLite and used for photopolymerization. The previous enamelRadii-cal. This fact is not in agreement with a etch may have guaranteed a higher bond perfor-previous study, which found that polywave LEDs mance due to the increase in the enamel surface freepromote better resin mechanical properties com- energy caused by a deeper enamel demineraliza-pared to single-peak LEDs, even when the light tion.4,5,14 The etching pattern of Clearfil Tri-S withcuring tip end is located at a long distance.22 previous acid treatment shows a deeper demineral- For half of the tested groups the thermomechan- ization of enamel cores and boundaries, favoring theical loading promoted higher gap formation, partial- penetration of the adhesive resin. Consequently, theFigure 4. (A): SEM photomicrograph showing the smooth enamel etching promoted by Clearfil Tri-S, with no dissolution of prism cores andboundaries. (B): SEM photomicrograph showing the smooth primer etching of Clearfil SE, with a type I etching pattern, with only dissolution of prismboundaries.
8 Operative Dentistry thermomechanical effect was not capable of inducing higher gaps at the interface, preserving the enamel/ composite bonding. For FL, the aging may not have affected bonding to enamel because this LCU emitted higher light irradiance compared to the other curing devices, even if the energy dose was standardized. This higher irradiance may have caused a bond disruption at the interface both before and after thermomechanical fatigue.32-34 For Clearfil SE, Ultra-Lume curing light promoted the maintenance of marginal integrity even after thermomechanical aging, regardless of additional enamel etching. This may be explained by the hydrophobic layer of this bond system which may have not been influenced by the composite shrinkage stress and consequently maintained the bond inter- face with no alterations. This additional layer can promote a higher monomer conversion and allow marginal integrity after thermomechanical loading. Also, when RD was used with enamel etching, the aging loading did not influence the percentage of marginal gaps. Although some in vitro studies exist, final conclu- sions regarding the role of enamel selective acid etching for self-etch adhesives in Class I composite restorations will depend on the outcomes of clinical trials. Clinical long-term studies and investigations of the retention ability of this approach for bond systems in the oral environment can best evaluate the quality and durability of these restorations. CONCLUSION Selective enamel etching promotes better marginal integrity for Clearfil Tri-S, showing itself to be an efficient additional step for Class I composite restorations. The two-step self-etch adhesive was not influenced by selective enamel etching or by the LED-curing unit. In general, the mild one-step self- etch bond system preserved the marginal adaptation integrity when enamel was previously etched, except when the single-peak LED FlashLite, with higher irradiance, was used. (Accepted 22, August 2011)Figure 5. (A): SEM photomicrograph of Clearfil Tri-S with previous REFERENCESphosphoric acid etching, showing a deep dissolution of prism coresand boundaries, with a type III etching pattern (characteristics of the 1. Ferracane JL (2011) Resin composite—State of the arttype I and II). The white arrows point to the characteristics of type I Dental Materials 27(1) 29-38.etching pattern, with intact prism core, while the black arrows showcharacteristics of the type II etching pattern, with higher dissolution of 2. Nikaido T, Kunzelmann KH, Chen H, Ogata M, Haradaprism peripheries. (B): SEM photomicrograph of Clearfil Tri-S with N, Yamaguchi S, Cox CF, Hickel R, Tagami J (2002)higher magnification 50003. (C) SEM photomicrograph of Clearfil SE Evaluation of thermal cycling and mechanical loading onwith previous acid etching, with a type III etching pattern, pointed out bond strength of a self-etching primer system to dentinby the white arrows. Dental Materials 18(3) 269-275.
Souza-Junior Others: Effect of Enamel Etching on Marginal Adaptation of Composite Restorations 9 3. Van Meerbeek B, De Munk J, Yoshida Y, Inoue S, Vargas 17. Bortolotto T, Onisor I, Krejci I (2007) Proximal direct M, Vijay P, Van Landuyt K, Lambrechts P, Vanherle G composite restorations and chairside CAD/CAM inlays: (2003) Buonocore memorial lecture. Adhesion to enamel Marginal adaptation of a two-step self-etch adhesive with and dentin: Current status and future challenges Oper- and without selective enamel conditioning Clinical Oral ative Dentistry 28(3) 215–235. Investigations 11(1) 35-43. ˜ 4. Perdigao J, Lopes MM, Gomes G (2008) In vitro 18. Wiggins KM, Hartung M, Althoff O, Wastian C, Mitra bonding performance of self-etch adhesives: II—Ultra- SB (2004) Curing performance of a new-generation light- morphological evaluation Operative Dentistry 33(5) emitting diode dental curing unit Journal of the American 534-549. Dental Association 135(10) 1471-1479. 5. Ermis RB, Temel UB, Celik EU, Kam O (2010) Clinical 19. Asmussen E, Peutzfeldt A (2003) Light-emitting diode performance of a two-step self-etch adhesive with addi- curing: Influence on selected properties of resin compos- tional enamel etching in Class III cavities Operative ites Quintessence International 34(1) 71-75. Dentistry 35(2) 147-155. 20. Hammesfahr PD, O’Connor MT, Wang X (2002) Light- 6. Peumans M, De Munk J, Van Landuyt KL, Poitevin A, curing technology: Past, present and future Compendium Lambrechts P, Van Meerbeek B (2010) Eight-year of Continuing Education in Dentistry 23(9 Supplement clinical evaluation of a 2-step self-etch adhesive with and 1) 18-24. without selective enamel etching Dental Materials 26(12) 1176-1184. 21. Antonson SA, Antonson DE, Hardigan PC (2008) Should my new curing light be an LED? Operative 7. Van Landuyt KL, Kanumilli P, De Munk J, Peumans M, Dentistry 33(4) 400-407. Lambrechts P, Van Meerbeek B (2006) Bond strength of a mild self-etch adhesive with and without prior acid- 22. Price RTB, Fahey J, Felix CM (2010) Knoop hardness of etching Journal of Dentistry 34(1) 77-85. five composites cured with single-peak and polywave LED curing lights Quintessence International 41(10) 8. Rotta M, Bresciani P, Moura SK, Grande RHM, Hilgert e181-e191. LA, Baratieri LN, Loguercio AD, Reis A (2007) Effects of phosphoric acid pretreatment and substitution of ´ 23. Camilotti V, Grullon PG, Mendonca JM, D’Alpino PHP, ¸ bonding resin on bonding effectiveness of self-etching Gomes JC (2008) Influence of different light curing units systems to enamel Journal of Adhesive Dentistry 9(6) on the bond strength of indirect resin composite restora- 537-546. tions Brazilian Oral Research 22(2) 164-169. 9. Watanabe T, Tsubota K, Takamizawa T, Kurokawa H, 24. Price RBT, McLeod ME, Feliz CM (2010) Quantifying Rikuta A, Miyazaki M (2008) Effect of prior acid etching light energy delivered to a Class I restoration Journal of on bonding durability of single-step adhesives Operative the Canadian Dental Association 76(23) 1-8. Dentistry 33(4) 426-433. 25. Brandt WC, Schneider LFJ, Frollini E, Correr-Sobrinho10. Erickson RL, Barkmeier WW, Kimmes NS (2009) Bond L, Sinhoreti MAC (2010) Effect of different photo- strength of self-etch adhesives to pre-etched enamel initiators and light curing units on degree of conversion of Dental Materials 25(10) 1187-1194. composites Brazilian Oral Research 24(3) 263-270. ˜11. Perdigao J, Monteiro P, Gomes G (2009) In vitro 26. Souza-Junior EJ, Prieto LT, Soares GP, Dias CT, Aguiar enamel sealing of self-etch adhesives Operative Dentistry FH, Paulillo LA (2010) The effect of curing light and 40(3) 225-233. chemical catalyst on the degree of conversion of two dual cured resin luting cements Lasers in Medical Science Nov12. Van Meerbeek B, Kanumilli P, De Munk J, Van Landuyt 23 [Epub ahead of print]. K, Lambrechts P, Peumans M (2005) A randomized controlled study evaluating the effectiveness of a two-step 27. Alvim HH, Alecio AC, Vasconcellos WA, Furlan M, self-etch adhesive with and without selective phosphoric- Oliveira JE, Sad JRC (2007) Analysis of camphorqui- acid etching of enamel Dental Materials 21(4) 375-383. none in composite resins as a function of shade Dental Materials 23(10) 1245-1249.13. Brackett MG, Brackett WW, Haisch LD (2006) Micro- leakage of Class V resin composites placed using self- 28. Alonso RCB, Correr GM, Cunha LG, Borges AFS, Puppin etching resins: Effect of prior enamel etching Quintes- Rontani RM, Sinhoreti MAC (2006) Dye staining gap sence International 37(2) 109-113. test: An alternative method for assessing marginal gap formation in composite restorations Acta Odontologica14. Frankenberger R, Lohbauer U, Roggendorf MJ, Nau- Scandinavica 64(3) 141-145. mann M, Taschner M (2008) Selective enamel etching reconsidered: Better than etch-and-rinse and self-etch? 29. Hilton TJ (2002) Can modern restorative procedures and Journal of Adhesive Dentistry 10(5) 339-344. materials reliably seal cavities? Part 2 American Journal of Dentistry 15(4) 279-289.15. Khosravi K, Ataei E, Mousavi M, Khodaeian N (2009) Effect of phosphoric acid etching of enamel margins on ¨ 30. Frankenberger R, Kramer N, Lohbauer U, Nikolaenko the microleakage of a simplified all-in-one and a self-etch SA, Reich SM (2007) Marginal integrity: Is the clinical adhesive system Operative Dentistry 34(5) 531-536. performance of bonded restorations predictable in vitro? Journal of Adhesive Dentistry 9(1) 107-116.16. Peumans M, De Munk J, Van Landuyt K, Lambrechts P, Van Meerbeek B (2007) Five-year clinical effectiveness 31. Blunk U, Zaslansky P (2010) Enamel margin integrity of a two-step self-etching adhesive Journal of Adhesive of Class I one-bottle all-in-one adhesives-based restora- Dentistry 9(1) 7-10. tions Journal of Adhesive Dentistry 13(1) 23-29.
10 Operative Dentistry32. Alonso RCB, Cunha LG, Correr GM, Puppin-Rontani RM, stress of composite resins Journal of Applied Oral Correr-Sobrinho L, Sinhoreti MAC (2006) Marginal Science: Revista FOB 16(4) 266-270. adaptation of composite restorations photoactivated by LED, plasma arc, and QTH light using low-modulus resin 34. Cunha LG, Alonso RCB, Pfeifer CSC, De Goes MF, ´ liners Journal of Adhesive Dentistry 8(4) 223-228. Ferracane JL, Sinhoreti MAC (2009) Effect of irradiance33. Cunha LG, Alonso RCB, Souza-Junior EJC, Neves A, and light source on contraction stress, degree of conversion Correr-Sobrinho L, Sinhoreti MAC (2008) Influence of and push-out Bond strength of composite restoratives the curing method on the post-polymerization shrinkage American Journal of Dentistry 22(3) 165-170.